Magnetic nanostructures are being developed for use in many aspects of our daily life, spanning areas such as data storage, sensing and biomedicine. Whereas patterned nanomagnets are traditionally two-dimensional planar structures, recent work is expanding nanomagnetism into three dimensions; a move triggered by the advance of unconventional synthesis methods and the discovery of new magnetic effects. In three-dimensional nanomagnets more complex magnetic configurations become possible, many with unprecedented properties. Here we review the creation of these structures and their implications for the emergence of new physics, the development of instrumentation and computational methods, and exploitation in numerous applications.
Nanomagnetism, the scientific field dedicated to the study of nanoscale magnetic objects, has undergone an explosion of activity over the last few decades, driven by fascinating discoveries such as the interaction of magnetization with spin currents (the area of spintronics)1,2 and a wide range of real-world applications3,4,5,6,7. For example, since both the storage and sensing parts of hard disk drives use nanomagnetic structures, the development of nanomagnetism has been a key factor in the vast recent improvements in computer performance and the development of cloud computing. With the exception of some self-assembled systems8,9, nanomagnetism has been mostly confined to two dimensions. In two-dimensional (2D) patterned planar single- or multi-layered magnetic structures, the thickness is of the order of some characteristic magnetic length-scale. This simple geometry leads to monodomain magnetic states in the vertical direction, restricting functionality to the substrate plane (Fig. 1b). In these cases, complex and useful magnetic behaviour is nevertheless possible by exploiting interfacial effects between layers.
The maturity now reached in this field10, together with the need for low energy technologies with new functionalities11 and the advent of advanced chemical and self-assembly synthesis techniques capable of growing non-planar nano-objects, make the expansion of nanomagnetism into three dimensions possible (Fig. 1a). In this new paradigm, spin configurations and capabilities extend not only in the plane but also into the vertical direction, and more complex, hierarchical systems leading to new effects can be designed. In this article, we review the state-of-the-art of three-dimensional (3D) nanomagnetism: the new physics associated with different types of 3D magnetic nanostructures, the most promising synthesis and characterization techniques available to create (Box 1) and probe (Box 2 and Box 3) these systems, and the latest advances in computational methods for their modelling (Box 4). We also highlight some of the major challenges still associated with these studies, and the great potential of this field to impact areas such as sensing, data storage, nanoelectronics, the Internet-of-Things and medical biology.
Emerging physics of 3D nanomagnetism
New types of domain walls
The extension of 2D nanostructures into the 3D world brings with it the emergence of unconventional spin textures, where novel physical effects comprising geometry, topology and chirality are involved. A paradigmatic example regards domain walls (DWs) in magnetic nanowires (NWs). NWs are subject to extensive investigation in nanomagnetism because of their potential use as DW conduits for memory and sensing applications12,13,14. Considering in detail NWs formed by soft magnetic materials, magnetization tends to be aligned parallel to their long direction, due to shape anisotropy. In this case, DWs are of either head-to-head or tail-to-tail type, holding a magnetostatic charge 2SMs (with S the NW section and Ms the spontaneous magnetization of the material), irrespective of the spin texture within the wall. This gives rise to magnetostatic energy, such that competition with exchange determines a complex panorama of DW types, in a manner depending on dimensionality and strip size. The size is compared with the characteristic dipolar exchange length Δd=(2A/μ0Ms2)1/2 (ref. 15), where A is the exchange stiffness of the material. We first describe their static features, before highlighting some peculiar aspects of their dynamics.
2D NWs (from now on denoted nanostrips to distinguish them from their 3D counterparts) have been widely studied in theory, simulation and experiments, because of their ease of fabrication and integration into devices. These are patterned with standard top–down lithography methods from thin films, having widths much larger than Δd and thicknesses comparable or not much larger than a few times this length. Thus, any significant variation of magnetization across thickness is prohibitively expensive energetically, such that magnetization textures can be faithfully described by a 2D field of a 3D magnetization vector M(x,y). For those nanostrips with moderate widths, significant variation of magnetization across the nanostrip would also be energetically unfavourable. Therefore, such DWs may be described using a 1D model by M(y), where magnetization in the core of the wall is aligned transverse to the strip long axis y; this is the so-called transverse DW (TDW, see Fig. 2a). Obviously, the transverse component imparts additional dipolar energy due to the edge charges that are created. For sufficiently wider strips, this energy can be reduced by the emergence of a different type of magnetic boundary, the vortex DW (VDW): here, magnetization becomes more parallel to the strip edge by curling around a vortex with core perpendicular to its surface (Fig. 2a). These two types of DWs share a large metastability region in the phase space, consisting of thickness (t) versus width (w), around an iso-energy line, determined by simulations16 as tw≃61Δd2.
To extend this already well understood phase diagram (see dashed region in Fig. 2b) to an arbitrary cross-section, the thickness of a nanostrip can be progressively increased towards a NW of square cross-section. DWs initially transverse and vortex in nature end up in magnetization textures with a tube of magnetization going through the wire along a transverse direction, x and z respectively. Remarkably, these two types of walls, characterized now by a full 3D magnetization field M(x,y,z), are identical upon rotation by π/2 around the wire axis. For large lateral wire dimensions, they display simultaneously transverse and vortex characteristics. They may, therefore, be denoted transverse-vortex domain walls (TVDWs)15, whereas the denotation of either transverse or vortex is sufficient in nanostrips (or π/2-rotated: very narrow and thick NWs), where one of these features is largely dominant (Fig. 2a). Being able to transform from one to the other using only continuous transformations from the flat nanostrips reveals that they share the same topology. This topological equivalence remains valid for any NW cross-sectional shape, for instance either square or circular.
Until now in our discussion, 3D NWs were considered as if the 2D DW magnetization was simply extruded along the third direction. However, considering 3D NWs from the start allows for the emergence of novel spin textures. The DWs so far described display two areas where magnetization is perpendicular to the wire surface: the entry and outlet points of the vortex core. Since magnetization pointing perpendicular to a surface implies an increase in magnetostatic energy, DW configurations with a more efficient magnetic flux closure (that is, with magnetization mostly parallel to the wire surface at any point) should be expected. Such a texture is possible for cylindrical symmetry, leading to a curling of the magnetization parallel to the wire axis. For a solid cylindrical NW, and with these boundary conditions, the continuity of a vector field of uniform magnitude becomes impossible17. Hence, there must exist one point where M cancels, that is, a local singularity where ferromagnetism is quenched. This very peculiar object, called a Bloch point, was theorised decades ago, based on similar external boundary conditions in bubble media18,19. It refers to a micromagnetic object of zero dimensions (0D); it is the counterpart of Bloch walls as 2D objects separating 3D domains. This wall, shown in Fig. 2a, is characterized by an axial vortex, that is, its axis is parallel to the wire, and with the Bloch point lying on the axis. It can accordingly be named a Bloch point DW (BPDW)20. Its existence was first predicted by means of micromagnetic simulations21,22. Taking these considerations into account, a general thickness-versus-width phase diagram reflecting the energetics of TVDWs and BPDWs in 3D NWs can be constructed (Fig. 2b). In the white and green regions of the diagram, the TVDW is the DW ground state, with either transverse or vortex features, respectively, becoming more evident for each area. The blue region, on the contrary, refers to the parameter space where the BPDW is the ground state, which occurs for lateral dimensions typically above 7Δd. It is worth noting that there exist large areas of this phase diagram where two or even three of these walls may coexist as (meta)stable states15. The first experimental imaging of TVDWs23,24 and BPDWs24 in NWs has recently been reported.
The above description of DWs in NWs illustrates characteristics of 3D spin textures displayed by other non-planar nanomagnetic objects. For instance, nanotubes (NTs) exhibit a rather similar phenomenology25, with just qualitative differences of the iso-energy lines, and notably with the absence of the Bloch points seen in the case of DWs with an axial vortex. The ends of elongated objects are also worthy of consideration, as they constitute the loci of nucleation for magnetization reversal. With the same physics (magnetostatics versus exchange) at play, these loci display end states called ‘C’ or curling, which may be viewed as a fraction of a TDW or BPDW, respectively22.
Additionally, unlike planar surfaces, curved surfaces lack space inversion symmetry. This can be the source of remarkable effects26. For instance, micromagnetic simulations have shown that the surface curvature in cylindrical NTs and NWs can give rise to a chiral symmetry breaking that results in different properties, depending on the rotation sense of the magnetization. This effect resembles the Dzyaloshinskii–Moriya interaction (DMI)26. To address this phenomenon of curvature-induced DMI, a 3D theory has recently been proposed27, consisting of reducing magnetostatic effects to an effective anisotropy. Under this assumption, curvature and torsion in NWs and shells split up the existing exchange interaction into scalar Heisenberg exchange and two effective magnetic interactions, namely curvature-induced effective anisotropy (magnetization patterning) and curvature-induced effective DMI (chirality selection)27,28. Systematic studies of magnetic NTs have proven the existence of an exchange energy that manifests as an effective easy-axis anisotropy along the tube axis25,29, which induce a gap in the dispersion relation of magnonic spin excitations in NTs30. Remarkably, the strength of the curvature-induced chiral effects could be tuned mechanically by bending flexible magnetic nanomembranes31, thereby providing a new method to manipulate magnetic properties at the nanoscale.
Dynamic magnetic properties may also differ significantly between 2D and 3D nanomagnets, as recently demonstrated in the case of DW propagation and NWs. The dynamic motion of DWs in NWs is of paramount importance for their exploitation in applications. This has led to a large amount of works in nanostrips in the last years20,32,33,34, where a complex scenario including several regimes of DW propagation, can be observed. In particular, DWs under external fields usually become unstable when propagating above a critical speed, an effect called Walker breakdown35. This effect originates from a torque exerted by the driving field on the DW. If this torque is sufficiently strong, the wall magnetic structure changes significantly in a periodic fashion, causing the motion to become oscillatory, as described by the Landau–Lifshitz–Gilbert equation20. Recent studies using micromagnetic simulations36,37 carried out in cylindrical NWs and NTs, reveal that DWs with an axial vortex configuration (BPDWs in the case of NWs) can propagate smoothly at very high speed (∼1 km s−1) when driven by an external magnetic field, overcoming the Walker breakdown36,38. Axial VDWs in NTs and NWs can surpass this limit due to the radial component of the magnetization36,37, caused by magnetostatic field distributions. This stability against the Walker breakdown in NTs and cylindrical NWs, described by micromagnetics, can also be understood in the context of the aforementioned chiral break of symmetry due to the surface curvature36. The effective dynamic-DMI counteracts this torque and thereby preserves the magnetic structure of the DW, even at large fields. Since this is a chiral effect, only one of the two possible vortex configurations of the DW is stabilised. These ultra-stable DWs can even reach the phase velocity of spin waves and thereby give rise to the Spin-Cherenkov Effect36 (Fig. 2c,d). This effect describes the spontaneous emission of spin waves occurring when a perturbation in a magnetic system moves faster than a threshold velocity, a phenomenon similar to sound waves generated by supersonic aircraft crossing the sound barrier. At these elevated velocities, DWs emit bichromatic spin waves of velocity-dependent wave length36.
Moreover, while the static structure of BPDWs in cylindrical NWs is now relatively well understood, the dynamic structure remains largely unexplored. This is because BPDWs are difficult to access experimentally and because the singularities of the magnetization field are characterized by a pronounced inhomogeneity of the magnetization that persists down to the atomistic scale, thereby making their simulation unreliable with standard micromagnetic codes. To resolve this problem, a hybrid atomistic-micromagnetic method has been recently developed with which the structure and the dynamics of BPDWs in NWs have been simulated at the atomic scale39, predicting a peculiar oscillation in the dynamics during field-driven motion40.
3D spin textures
3D magnetic spin textures with non-trivial topological charges (vortices, skyrmions and chiral bubbles) possess an exceptional stability under external perturbations against transitions into trivial states, for example, to collinear magnetization. Enhanced stability, particle-like properties and high susceptibility to electric, spin and heat currents, and magnonic excitations have put these chiral structures into the spotlight of fundamental sciences, as well as application-oriented research. A paradigmatic 3D spin texture is the magnetic vortex with its nanometric core magnetization (Fig. 3a). Experimentally observed for the first time almost two decades ago41, it is typically present in patterned thin films formed by soft magnetic materials. The spin structure is defined by both in-plane magnetic circulation and out-of-plane core polarity, with the core expanding laterally ∼10 nm42, as set by Δd. This strong confinement has allowed the quantification of pinning site potentials in thin films by probing Barkhausen noise43, generate nano- and micro-oscillators with tuneable frequency44 and design of magnetic vortex memories45.
While the chirality of vortices (defined as the product of circulation and core polarity) and other objects such as Bloch points is intrinsically degenerate in common 2D nanomagnets, 3D geometries with inherent new types of interactions can break this symmetry. As mentioned above, this is the case of 3D curved nanomagnets, which reveal a chirality selection due to curvature-driven DMI46. Similarly, heterostructures formed by ultrathin magnetic thin films and heavy-element materials with large spin–orbit coupling, result in interfacial antisymmetric spin couplings due to spin-polarized scattering from conduction electrons in the heavy-element layer. This antisymmetric exchange interaction, referred to as interfacial DMI (IDMI)47, favours non-collinear chiral spin configurations. The competition of IDMI with standard symmetric exchange interactions (that is, Heisenberg and Ruderman–Kittel–Kasuya–Yosida (RKKY)), as well as magnetic anisotropies, results in a very rich magnetic phenomenology48, including in some cases the presence of magnetic skyrmions (Fig. 3b). Skyrmions are topologically protected 3D spin textures which subtend the whole 4π steradians of the spin space with a resulting non-trivial integer topological charge. They may exist as truly localized solitary objects with continuous magnetization rotation. For the formation of skyrmion lattices, large IDMI values, and typically magnetic bias fields are needed. The magnitude of IDMI depends significantly on the electron orbit overlap, and thus on the film elements, their arrangement, temperature and strain. Except in some special cases49, IDMI is typically orders of magnitude lower than the symmetric exchange interactions, with its effective value decreasing with magnetic film thickness50. In films with smaller IDMI, this is nevertheless enough to break the inversion symmetry and select one of the two possible DW chiralities51, forming, for example, chiral bubbles (Fig. 3c).
Following the first theoretical predictions and experimental evidence of skyrmions in single-phase bulk magnetic materials with non-centrosymmetric crystallographic structures, research activities are now mostly focused on heterostructures with IDMI, due to their potential for applications52. Crucial aspects, such as creation, detection, manipulation and deletion of individual nanoscale skyrmions were first shown in Pd/Fe bilayers on Ir(111) utilizing spin-polarized scanning tunnelling microscopy53. The strong IDMI in single Fe monolayers on Ir(111) stabilizes a non-reconfigurable skyrmion lattice that exists for temperatures up to 30 K and magnetic fields up to 9 T. The stabilization of skyrmions at room temperature has been achieved by increasing the film thickness of the transition metal, providing interlayer exchange interaction, and engineering asymmetric multilayer stacks with distinct heavy-element films for additive IDMI at top and bottom interfaces of the magnetic layer54. The corresponding skyrmion core/bubble size at room temperature is on the order of 10–100 nm54,55, and hence 10–100 times larger than those in Fe/Ir(111).
Owing to their small size, highly non-collinear spin texture and topological protection, they can act as localized mobile data for spintronic applications. To write, read and delete these skyrmions/chiral bubbles, several mechanisms have been proposed and some demonstrated. These include spin-transfer/spin–orbit torque via spin-polarized current, magnons, spin Hall effect and electric field-driven magnetoelectric coupling53,56,57,58. The potentially low pinning and small scattering cross-section of skyrmions originating from their spatial confinement implies both small on-set current density and large lateral deflection due to an accompanying Magnus force59. Current-independent unidirectional motion along nanostrips may be enforced via strain, exchange or anisotropy modulations58, or eventually considering antiferromagnetic (AF) skyrmions60. In practice, pinning/scattering at grain boundaries caused by structural and magnetic imperfection in polycrystalline and amorphous films results in larger current densities required for coherent motion54.
Vertical data motion using magnetic solitons
The extension of magnetic data mobility to the vertical direction has been recently realised by means of magnetic solitons in AF superlattices; this opens a new route to 3D magnetic random access memory devices with out-of-plane functionality. The term soliton refers here to a (topological) kink in a discrete chain of spins61, and is equivalent to an AF wall. The idea is analogous to the one employed in Nano-Magnetic Logic62, but instead of using soliton motion in dipolar-coupled nanomagnets positioned on the substrate plane, solitons are moved perpendicularly to the substrate plane in magnetic superlattices, where the coupling between magnetic thin films is provided by non-magnetic spacers via AF RKKY interactions. The system can be represented in its simple form by a 1D chain of spins (Fig. 3d), following a macrospin approximation, where layer thickness (t), anisotropy (K) and surface coupling (J) energies rule the physics of the system. Depending on the ratio between RKKY coupling and anisotropy fields (HJ=|J|/(μ0Mst) and Hu=2 K/(μ0Ms) respectively) three regimes regarding magnetic texture and motion of solitons can be distinguished, as schematically shown in Fig. 3d.
For high RKKY couplings, solitons are wide, comprising a large number of layers, with those spins forming the soliton deviating a great amount from the anisotropy direction. In systems with very high coupling/anisotropy ratios, the rotation results in helical spin structures63. For soliton nucleation, the surface-spin flop transition can be exploited64, and reliable unidirectional propagation can be achieved by creating asymmetric superlattices, where thickness and anisotropy of a gate edge layer is tuned differently from the others. Following this approach, asynchronous motion under external magnetic fields using gates formed by single65 and highly coupled multiple layers66 has been achieved. As RKKY coupling decreases, becoming comparable to anisotropy, solitons get narrower, acquiring a well-defined magnetic moment. Interestingly, macrospin and micromagnetic simulations predict how in this case, external rotating magnetic fields can couple to the soliton magnetic configuration, resulting in synchronous propagation with the field, where the direction of motion is defined by the soliton chirality and sense of rotation of the field. This could be exploited to create bi-directional multi-bit vertical shift registers67.
Moreover, in spite of losing their chirality, synchronous motion is also possible for sharp solitons (when anisotropy becomes much larger than coupling). This has been realised under external oscillating magnetic fields, in Ising systems with strong perpendicular magnetic anisotropy, where the intrinsic layer coercivity (Hc) substitutes Hu as relevant parameter for operation. By carefully engineering the thickness of the layers and the exchange coupling between them, it is possible to break inversion symmetry, which induces a unidirectional ratchet action68. Figure 3e shows schematically the structure of a ratchet superlattice, where layer thickness and interlayer RKKY coupling oscillate periodically between two possible values. Such a scheme makes possible the synchronous propagation of a soliton with perpendicular oscillating magnetic fields68. Remarkably, and following this approach, a unidirectional soliton shift register with vertical functionality equivalent to ∼20 transistors has been achieved within a thickness of 2 nm (ref. 68). Simple logic operations involving soliton–soliton annihilation have been realised as well69. Analogous ratchet schemes are possible; for example, a similar behaviour has been achieved by designing a superlattice with same thickness for all magnetic layers, and a combination of AF and ferromagnetic interlayer couplings70.
The aforementioned results refer to studies in extended films. Future studies are expected in laterally patterned nanostructures, to investigate the effect of rotating fields and dipolar interactions on the domain formation and soliton operation71,72. The use of different mechanisms for propagation, such as spin-transfer torque73, microwave excitations74 or all optical switching75, are also anticipated. Additionally, a new energy storage concept based on the continuous injection of solitons via the rotation of one edge spin in a cork-screw fashion, has been recently proposed63.
Future applications of 3D nanomagnetism
Sensing and actuation
The use of 3D nanomagnets for sensing and actuation applications has a huge potential in many scientific and technological areas. Some of the novel functionalities foreseen in the field of 3D magnetic nano-sensing are the substantial increase in surface-to-volume ratio with respect to planar systems, their capability to probe vectorial fields, an ad hoc geometrical design to match a sensed structure, and the exploitation of mechanical and thermal effects present in suspended structures which may couple to their magnetic response.
In particular, 3D magnetic nanomembranes (forming part of the large family of emerging flexible devices, for example, electronics displays and solar cells) which are transforming rigid electronics into light and shapeable elements, have already proven to bear great universal potential as flexible magnetic sensors. Remarkably, their magnetic sensitivity, harnessing giant magnetoresistance or giant magnetoimpedance, is similar (or in some cases more than one order of magnitude larger76) to devices produced on Si wafers, even after demanding manipulations4,77. This is due to the continuity of the magnetization along their closed surface, that is, due to their topology78. These features have stimulated desire for their application in industry as precise and flexible positioning control of magnetic bearings in electric motors79, and as printable sensing paste for simple but versatile magnetic switches (for example, electric postcards80). Further potential applications in life sciences and diagnostics include light, mobile and affordable devices with great spatial localization so as to facilitate magnetoencephalography76 for early stage disease detection.
Additionally, 3D nanomagnets could be incorporated as sensors in a new generation of scanning probe microscopy methods for advanced imaging and spectroscopy. In fact, high aspect-ratio NWs have already been employed as ultra-sharp MFM tips, improving magnetic resolution down to 10 nm81 and overcoming limitations of standard triangular tips in probing 3D nanostructures82. Furthermore, nano-spheres grown on top of cantilevers have been exploited to perform ferro-magnetic-resonant force microscopy, measuring magnetization dynamics with high spatial resolution83. The development of new tip designs incorporating new geometries and materials can exploit high-order resonant cantilever modes to measure field gradient components along several directions in space84. This and other approaches85 could make possible the realization of scanning probe vectorial microscopy: mapping the three components of stray fields emanating from a magnetic system at nanoscale resolution.
Moreover, 3D nanostructures often make very good actuators: their larger volume compared to planar 2D structures increases the torque and force generated by electromagnetic fields and strain. They are often free to deform reversibly, with interest for the NEMS industry, nanoelectronics, sensing, robotics and studies in the quantum regime86,87,88,89,90. In the case of 3D nanomagnets, additionally to standard electrical driving methods, remote magnetic actuation is possible via external magnetic fields91. This can be exploited to create nanomotors in fluids, where chiral helical structures92 or Janus particles93 have been controllably moved under rotating and oscillating magnetic fields, respectively. We foresee future works exploiting dipolar interactions, integrating different magnetic materials and more complex geometries, incorporating optical and electrical readout methods, and further integration into biological environments.
In particular, 3D nano- and micro-scale mechanical actuators are a key part of the tool-kit of mechano-biology94,95, an emerging field which tries to understand the role of cell and tissue mechanics in diseases. Single 3D magnetic nanostructures subjected to laboratory-scale magnetic fields can generate tens of nanonewton of force locally and controllably to cells. This is sufficient to probe the phenotype of cells96, mechanically induce differentiation of bone stem cells97, burst payload-carrying neural stem cells98 and destroy cancer cells99. Additionally, mammals use motile cilia (flagella-like microtubules) beating together to sweep objects through organs (such as removing dirt from the lungs or transporting eggs through female Fallopian tubes). Magnetic NWs could perhaps form artificial cilia100, transporting reagents through on-chip microfluidic channels.
Towards data storage and the Internet-of-Things
3D magnetic nanostructures could form the basis of a new storage class of non-volatile memories, in which multiple data bits are stored magnetically above a single electronic memory cell on an integrated circuit. This is sustained by the impressive progress on ‘magnetic data mobility’ in the last few years, in which physical effects such as spin-transfer torque101,102 allow digital information to be propagated through nanomagnets via magnetic entities such as DWs, skyrmions or solitons. The realization of 3D magnetic memories could be implemented using perhaps the original racetrack architecture103. Alternatively, existing magnetic random access memory technology could be enhanced by increasing the number of data storing magnetic layers in the stack, such that each cell can store a data word instead of a data bit104. In both of these cases, digital shift-register action is an essential ingredient68, allowing data bits in magnetic form to be sequentially pumped into the nanomagnet during writing and then pumped back out during reading. Also, a recent trend in microelectronics is to create 2.5-dimensional devices105 by stacking multiple thin substrates on top of each other in a single package, with wire interconnects running between layers. Magnetic NWs could use these ideas to enable 2.5-dimensional spintronic devices (that is, chips which use both electronic and magnetic components), allowing chip designers to connect electronic parts using electrical wires and magnetic parts using magnetic NWs.
Magnetic interconnect is a particularly interesting idea because it can host both magnetic DWs106 and magnetic spin waves107. The former would carry digital information in a very compact form but at low speed, while the latter would offer long-range transmission. Intriguingly, the magnetic hysteresis and non-linearity present in many magnetic NWs mean that the interconnect is potentially also both a memory element and a logic gate108, opening up new computing architectures in which the traditional boundaries between memory, logic and interconnect are eliminated. Such chips could even go beyond conventional Boolean logic and implement neuromorphic computing architectures109 in which 3D networks of magnetic NWs mimic the neurons and synapses in living brains.
However, significant challenges still remain before such applications become reality. In particular, modern microelectronics makes great use of precision interfaces between materials; many of the growth techniques used for 3D structures do not currently offer sufficient purity and control to engineer interfaces with single atomic layer precision. Also, while planar microchips successfully integrate and connect 108 transistors on a single chip, complex interconnectivity in 3D is still to be developed. A human brain may connect up to 104 synapses to each neuron110; there are currently no known 3D fabrication techniques able to achieve this.
The integrated circuits of the future will increasingly incorporate a wider range of technologies onto a single die to form full systems (Fig. 4). The inclusion of physical sensors and energy harvesters into the menu of devices available to designers is particularly important for the Internet-of-Things. 3D magnetic nanostructures may find a role in both of these, where large surface areas, the ability to easily strain, and the possibility of sustaining temperature differentials are often important and difficult to achieve in 2D planar geometries. Recent advances in spin caloritronics111 and multiferroic materials112 will provide the necessary interconversion between the electronic, magnetic and thermal worlds.
The move from 2D to 3D is not only a current trend within nanomagnetism, but is part of a wider theme within nanotechnology in general. Nanoelectronics, nanophotonics, energy storage and harvesting, and nanomedicine, all stand to benefit from a new era of greener, more capable, multi-functional technologies brought about by moving into the third dimension. Despite the great challenges ahead, recent advances in bottom-up lithography, microscopy and computational techniques make its future realization feasible.
3D nanomagnetism, still in its infancy, needs to fulfil key milestones in the future. The experimental realization of spintronic devices requires high-quality materials, for example, DW motion may be severely affected by the presence of defects. Achieving such a quality with unconventional synthesis methods is still work in progress. Also, next-generation 3D nanomagnets will require advanced magnetic materials such as Heusler alloys, multi-layered and epitaxial thin films, and highly functional interfaces. These barriers could be overcome using fabrication strategies which combine multiple synthesis techniques, including innovative ways to exploit differential strain113. The low throughput currently achievable in 3D nano-printing could be significantly enhanced by moving from the gas phase to the liquid phase114. This may enable the development of complex architectures, mass fabrication and the creation of multi-functional designs. Future years will also see rapid progress in the synthesis of novel magnetic materials such as 3D nanocomposites115, where strong electric fields at interfaces or magnetostrictive effects could be used for energy harvesting. Magnetic tools able to probe 3D nanomagnets are essential as well. Vectorial magnetometry and magnetic microscopy of nanostructures require a phenomenal combined effort comprising instrumentation, electronics and data analysis. Recent progress in magnetic microscopy methods116,117,118,119, pushing further spatial and temporal resolution, is expected to bring new opportunities in this area. An essential cornerstone still missing due to its technical complexity is the development of methodologies120 to electrically contact individual 3D nano-geometries.
Advances in these areas are essential to study 3D spin textures further. Recent experimental work has confirmed theoretical and computational predictions about their magnetic structure and static behaviour. The next step is now to focus on the experimental realization of specific dynamic features driven by different mechanisms. These are often related to the interplay between the chirality and/or curvature of the boundaries of the texture itself and the chiral nature of the Landau–Lifshitz equation. Interest is also growing in composite spin textures such as coupled bilayers121, where flux closure and moment compensation can enhance magnetic DW motion within the plane, as well as leading to motion between horizontal planes. The search for and realization of ever more complex geometries will continue, for example, by connecting planar and vertical structures, creating core-shell 3D objects, or exploiting topological effects via the interplay between 3D shapes and spin configurations122. The possibility of creating complex 3D networks of nanomagnets could lead to new computational paradigms123, and is also expected to elucidate open questions regarding effects involving numerous interacting magnetic particles, for example, artificial spin-ice lattices124. Three-dimensional nanomagnetism, with its vast amount of unexplored science and huge potential to impact society, is a fascinating new research area, which will flourish in the years to come.
How to cite this article: Fernández-Pacheco, A. et al. Three-dimensional nanomagnetism. Nat. Commun. 8, 15756 doi: 10.1038/ncomms15756 (2017).
Publisher’s note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Editorial. Memory with a spin. Nat. Nanotechnol. 10, 185–185 (2015).
Hoffmann, A. & Bader, S. D. Opportunities at the frontiers of spintronics . Phys. Rev. Appl. 4, 047001 (2015).
McCray, W. P. How spintronics went from the lab to the iPod. Nat. Nanotechnol. 4, 2–4 (2009).
Melzer, M. et al. Imperceptible magnetoelectronics. Nat. Commun. 6, 6080 (2015).
Makarov, D., Melzer, M., Karnaushenko, D. & Schmidt, O. G. Shapeable magnetoelectronics. Appl. Phys. Rev. 3, 011101 (2016).
Koh, I. & Josephson, L. Magnetic nanoparticle sensors. Sensors 9, 8130–8145 (2009).
Chen, R., Romero, G., Christiansen, M. G., Mohr, A. & Anikeeva, P. Wireless magnetothermal deep brain stimulation. Science 347, 1477–1480 (2015).
Faure, B. et al. 2D to 3D crossover of the magnetic properties in ordered arrays of iron oxide nanocrystals. Nanoscale 5, 953–960 (2013).
Sun, H. et al. Self-organized honeycomb structures of Mn 12 single-molecule magnets. J. Phys. Chem. B 113, 14674–14680 (2009).
Stamps, R. L. et al. The 2014 magnetism roadmap. J. Phys. D Appl. Phys. 47, 333001 (2014).
Waldrop, M. M. The chips are down for Moore’s law. Nature 530, 144–147 (2016).
Parkin, S. & Yang, S.-H. Memory on the racetrack. Nat. Nanotechnol. 10, 195–198 (2015).
Mattheis, R., Glathe, S., Diegel, M. & Hübner, U. Concepts and steps for the realization of a new domain wall based giant magnetoresistance nanowire device: From the available 24 multiturn counter to a 212 turn counter. J. Appl. Phys. 111, 113920 (2012).
Hrkac, G., Dean, J. & Allwood, D. A. Nanowire spintronics for storage class memories and logic. Philos. Trans. A Math. Phys. Eng. Sci. 369, 3214–3228 (2011).
Jamet, S., Rougemaille, N., Toussaint, J. C. & Fruchart, O. in Magnetic nano- and microwires: design, synthesis, properties and applications (ed. Vazquez M. 783–811Woodhead (2015).
McMichael, R. D., Eicke, J., Donahue, M. J. & Porter, D. G. Domain wall traps for low-field switching of submicron elements. J. Appl. Phys. 87, 7058–7060 (2000).
Arrott, A., Heinrich, B. & Aharoni, A. Point singularities and magnetization reversal in ideally soft ferromagnetic cylinders. IEEE Trans. Magn. 15, 1228–1235 (1979).
Feldtkeller, E. Mikromagnetisch stetige und unstetige Magnetisierungskonfigurationen. Z. Angew. Phys. 19, 530–536 (1965).
Malozemoff, A. P., Slonczewski, J. C. & Raymond, W. Magnetic Domain Walls In Bubble Materials Academic Press (1979).
Thiaville, A. & Nakatani, Y. in Spin Dynamics in Confined Magnetic Structures III eds Hillebrands B., Thiaville A. 161–205Springer (2006).
Forster, H. et al. Domain wall motion in nanowires using moving grids (invited). J. Appl. Phys. 91, 6914–6919 (2002).
Hertel, R. Computational micromagnetism of magnetization processes in nickel nanowires. J. Magn. Magn. Mater. 249, 251–256 (2002).
Biziere, N. et al. Imaging the fine structure of a magnetic domain wall in a Ni nanocylinder. Nano Lett. 13, 2053–2057 (2013) This paper demonstrates imaging of the internal structure of domain walls in cylindrical nanowires.
Da Col, S. et al. Observation of Bloch-point domain walls in cylindrical magnetic nanowires. Phys. Rev. B 89, 180405 (2014) This article reports experimental proof of the existence of Bloch-point domain walls in cylindrical nanowires.
Landeros, P. et al. Reversal modes in magnetic nanotubes. Appl. Phys. Lett. 90, 102501 (2007).
Hertel, R. Curvature-induced magnetochirality. SPIN 3, 1340009 (2013) This work presents a theoretical discussion of magnetochiral effects induced by surface curvature in ferromagnetic systems.
Gaididei, Y., Kravchuk, V. P. & Sheka, D. D. Curvature effects in thin magnetic shells. Phys. Rev. Lett. 112, 257203 (2014).
Sheka, D. D. et al. Curvature effects in statics and dynamics of low dimensional magnets. J. Phys. A Math. Theor. 48, 125202 (2015).
Landeros, P. & Nüńez, A. S. Domain wall motion on magnetic nanotubes. J. Appl. Phys. 108, 033917 (2010).
González, A. L., Landeros, P. & Núñez, Á. S. Spin wave spectrum of magnetic nanotubes. J. Magn. Magn. Mater. 322, 530–535 (2010).
Streubel, R. et al. Magnetism in curved geometries. J. Phys. D Appl. Phys. 49, 363001 (2016) A comprehensive topical review of 3D curved magnetic geometries.
Ryu, K.-S., Thomas, L., Yang, S.-H. & Parkin, S. Chiral spin torque at magnetic domain walls. Nat. Nanotechnol. 8, 527–533 (2013) This article provides an elucidation of the mechanisms behind chiral spin torques in nanostrips made of ultra-thin films.
Emori, S., Bauer, U., Ahn, S.-M., Martinez, E. & Beach, G. S. D. Current-driven dynamics of chiral ferromagnetic domain walls. Nat. Mater. 12, 611–616 (2013) This article demonstrates chiral spin torque in Neel-type domain walls in nanostrips.
Miron, I. M. et al. Fast current-induced domain-wall motion controlled by the Rashba effect. Nat. Mater. 10, 419–423 (2011).
Schryer, N. L. & Walker, L. R. The motion of 180° domain walls in uniform dc magnetic fields. J. Appl. Phys. 45, 5406–5421 (1974).
Yan, M., Andreas, C., Kákay, A., Garcïa-Sänchez, F. & Hertel, R. Fast domain wall dynamics in magnetic nanotubes: suppression of Walker breakdown and Cherenkov-like spin wave emission. Appl. Phys. Lett. 99, 122505 (2011) This numerical study predicts the Spin-Cherenkov effect in nanotubes.
Yan, M., Andreas, C., Käkay, A., Garcïa-Sänchez, F. & Hertel, R. Chiral symmetry breaking and pair-creation mediated Walker breakdown in magnetic nanotubes. Appl. Phys. Lett. 100, 252401 (2012).
Hertel, R. Ultrafast domain wall dynamics in magnetic nanotubes and nanowires. J. Phys. Condens. Matter 28, 483002 (2016).
Andreas, C., Kákay, A. & Hertel, R. Multiscale and multimodel simulation of Bloch-point dynamics. Phys. Rev. B 89, 134403 (2014) An application of multiscale modelling for the study of 3D spin textures.
Hertel, R. & Andreas, C. in Magnetic Nano- and Microwires. Design, Synthesis, Properties and Applications ed. Vazquez M. 653–677Woodhead (2015).
Shinjo, T., Okuno, T., Hassdorf, R., Shigeto, K. & Ono, T. Magnetic vortex core observation in circular dots of permalloy. Science 289, 930–932 (2000) This paper describes the experimental observation of vortices in dots.
Wachowiak, A. et al. Direct observation of internal spin structure of magnetic vortex cores. Science 298, 577–580 (2002).
Burgess, J. A. J. et al. Quantitative magneto-mechanical detection and control of the barkhausen effect. Science 339, 1051–1054 (2013).
Streubel, R., Fischer, P., Kopte, M., Schmidt, O. G. & Makarov, D. Magnetization dynamics of imprinted non-collinear spin textures. Appl. Phys. Lett. 107, 112406 (2015).
Zhu, J.-G., Zheng, Y. & Prinz, G. A. Ultrahigh density vertical magnetoresistive random access memory (invited). J. Appl. Phys. 87, 6668 (2000).
Pylypovskyi, O. V. et al. Coupling of chiralities in spin and physical spaces: the möbius ring as a case study. Phys. Rev. Lett. 114, 197204 (2015).
Zhang, S., Levy, P. & Fert, A. Mechanisms of spin-polarized current-driven magnetization switching. Phys. Rev. Lett. 88, 236601 (2002).
Bode, M. et al. Chiral magnetic order at surfaces driven by inversion asymmetry. Nature 447, 190–193 (2007).
Dupé, B. et al. Tailoring magnetic skyrmions in ultra-thin transition metal films. Nat. Commun. 5, 101–103 (2014).
Nembach, H. T., Shaw, J. M., Weiler, M., Jué, E. & Silva, T. J. Linear relation between Heisenberg exchange and interfacial Dzyaloshinskii–Moriya interaction in metal films. Nat. Phys. 11, 825–829 (2015).
Chen, G. et al. Tailoring the chirality of magnetic domain walls by interface engineering. Nat. Commun. 4, 2671 (2013).
Wiesendanger, R. et al. Nanoscale magnetic skyrmions in metallic films and multilayers: a new twist for spintronics. Nat. Rev. Mater. 1, 16044 (2016).
Romming, N. et al. Writing and deleting single magnetic skyrmions. Science 341, 636–639 (2013).
Woo, S. et al. Observation of room-temperature magnetic skyrmions and their current-driven dynamics in ultrathin metallic ferromagnets. Nat. Mater. 15, 501–506 (2016) This work reports the creation of skyrmions at room temperature, driven by current pulses in magnetic racetracks.
Jiang, W. et al. Blowing magnetic skyrmion bubbles. Science 349, 283–286 (2015) This article demonstrates injection and motion of skyrmionic bubbles at room temperature.
Hanneken, C. et al. Electrical detection of magnetic skyrmions by tunnelling non-collinear magnetoresistance. Nat. Nanotechnol. 10, 1039–1042 (2015).
Seki, S., Yu, X. Z., Ishiwata, S. & Tokura, Y. Observation of skyrmions in a multiferroic material. Science 336, 198–201 (2012).
Hsu, P.-J. et al. Electric field driven switching of individual magnetic skyrmions. Nat. Nanotechnol. 12, 123–126 (2017).
Reichhardt, C. & Reichhardt, C. J. O. Noise fluctuations and drive dependence of the skyrmion Hall effect in disordered systems. New J. Phys. 18, 095005 (2016).
Barker, J. & Tretiakov, O. A. Static and dynamical properties of antiferromagnetic skyrmions in the presence of applied current and temperature. Phys. Rev. Lett. 116, 147203 (2016).
Cowburn, R. P. Room temperature magnetic quantum cellular automata. Science 287, 1466–1468 (2000) This paper shows transport of magnetic information in isolated dots for nanomagnetic logic applications.
Niemier, M. T. et al. Nanomagnet logic: progress toward system-level integration. J. Phys. Condens. Matter 23, 493202 (2011).
Vedmedenko, E. Y. & Altwein, D. Topologically protected magnetic helix for all-spin-based applications. Phys. Rev. Lett. 112, 017206 (2014).
te Velthuis, S., Jiang, J., Bader, S. & Felcher, G. Spin flop transition in a finite antiferromagnetic superlattice: evolution of the magnetic structure. Phys. Rev. Lett. 89, 127203 (2002).
Fernández-Pacheco, A. et al. Controllable nucleation and propagation of topological magnetic solitons in CoFeB/Ru ferrimagnetic superlattices. Phys. Rev. B Condens. Matter Mater. Phys. 86, 104422 (2012).
Fernández-Pacheco, A. et al. Magnetic state of multilayered synthetic antiferromagnets during soliton nucleation and propagation for vertical data transfer. Adv. Mater. Interfaces 3, 1600097 (2016).
Petit, D., Mansell, R., Fernández-Pacheco, A., Lee, J. H. & Cowburn, R. P. in VLSI: Circuits for Emerging Applications ed. Wojcicki T. Ch. 12, CRC Press (2014).
Lavrijsen, R. et al. Magnetic ratchet for three-dimensional spintronic memory and logic. Nature 493, 647–650 (2013) This article presents the development of soliton-based vertical shift registers.
Lavrijsen, R. et al. Multi-bit operations in vertical spintronic shift registers. Nanotechnology 25, 105201 (2014).
Mansell, R. et al. A robust soliton ratchet using combined antiferromagnetic and ferromagnetic interlayer couplings. Appl. Phys. Lett. 106, 092404 (2015).
Lee, J. H. et al. Soliton propagation in micron-sized magnetic ratchet elements. Appl. Phys. Lett. 104, 232404 (2014).
Lee, J.-H. et al. Domain imaging during soliton propagation in a 3D magnetic ratchet. SPIN 3, 1340013 (2013).
Kudo, K. et al. Resonant magnetization switching induced by spin-torque-driven oscillations and its use in three-dimensional magnetic storage applications. Appl. Phys. Express 8, 103001 (2015).
Suto, H. et al. Three-dimensional magnetic recording using ferromagnetic resonance. Jpn J. Appl. Phys. 55, 07MA01 (2016).
Lambert, C.-H. et al. All-optical control of ferromagnetic thin films and nanostructures. Science 345, 1337–1340 (2014).
Karnaushenko, D. et al. Self-assembled on-chip-integrated giant magneto-impedance sensorics. Adv. Mater. 27, 6582–6589 (2015).
Melzer, M. et al. Stretchable magnetoelectronics. Nano Lett. 11, 2522–2526 (2011).
Makarov, D., Ortix, C. & Baraba, L. Functional magnetic nanomembranes. SPIN 3, 1302001 (2013).
Ernst, D. et al. Packaging technologies for (Ultra-)thin sensor applications in active magnetic bearings. in Proceedings of the 2014 37th International Spring Seminar on Electronics Technology 125–129IEEE (2014).
Karnaushenko, D., Makarov, D., Yan, C., Streubel, R. & Schmidt, O. G. Printable giant magnetoresistive devices. Adv. Mater. 24, 4518–4522 (2012).
Belova, L. M., Hellwig, O., Dobisz, E. & Dan Dahlberg, E. Rapid preparation of electron beam induced deposition Co magnetic force microscopy tips with 10 nm spatial resolution. Rev. Sci. Instrum. 83, 093711 (2012).
Gavagnin, M. et al. Free-standing magnetic nanopillars for 3D nanomagnet logic. ACS Appl. Mater. Interfaces 6, 20254–20260 (2014).
Guo, F., Belova, L. M. & McMichael, R. D. Spectroscopy and imaging of edge modes in permalloy nanodisks. Phys. Rev. Lett. 110, 017601 (2013).
Mühl, T. et al. Magnetic force microscopy sensors providing in-plane and perpendicular sensitivity. Appl. Phys. Lett. 101, 112401 (2012).
Schuhl, A., Gaudin, G., Sabon, P., Zermatten, P.-J. & Montaigne, F. Integrated magnetometer and its manufacturing process. World Patent Organization patent WO/2011/092406 (2011).
Blick, R. H., Qin, H., Kim, H.-S. & Marsland, R. A nanomechanical computer—exploring new avenues of computing. New J. Phys. 9, 241–241 (2007).
Chaste, J. et al. A nanomechanical mass sensor with yoctogram resolution. Nat. Nanotechnol. 7, 301–304 (2012).
Hanay, M. S. et al. Inertial imaging with nanomechanical systems. Nat. Nanotechnol. 10, 339–344 (2015).
Hanay, M. S. et al. Single-protein nanomechanical mass spectrometry in real time. Nat. Nanotechnol. 7, 602–608 (2012).
Aspelmeyer, M., Kippenberg, T. J. & Marquardt, F. Cavity optomechanics. Rev. Mod. Phys. 86, 1391–1452 (2014).
Vavassori, P., Pancaldi, M., Perez-Roldan, M. J., Chuvilin, A. & Berger, A. Remote magnetomechanical nanoactuation. Small 12, 1013–1023 (2016).
Walker, D., Kübler, M., Morozov, K. I., Fischer, P. & Leshansky, A. M. Optimal length of low reynolds number nanopropellers. Nano Lett. 15, 4412–4416 (2015).
Baraban, L. et al. Fuel-free locomotion of janus motors: magnetically induced thermophoresis. ACS Nano 7, 1360–1367 (2013).
Wheeler, M. A. et al. Genetically targeted magnetic control of the nervous system. Nat. Neurosci. 19, 756–761 (2016).
Kilinc, D., Dennis, C. L. & Lee, G. U. Bio-nano-magnetic materials for localized mechanochemical stimulation of cell growth and death. Adv. Mater. 28, 5672–5680 (2016).
Wang, N. & Ingber, D. E. Probing transmembrane mechanical coupling and cytomechanics using magnetic twisting cytometry. Biochem. Cell Biol. 73, 327–335 (1995).
Cartmell, S. H., Dobson, J., Verschueren, S. B. & El Haj, A. J. Development of magnetic particle techniques for long-term culture of bone cells with intermittent mechanical activation. IEEE Trans. Nanobiosci. 1, 92–97 (2002).
Muroski, M. E. et al. Controlled payload release by magnetic field triggered neural stem cell destruction for malignant glioma treatment. PLoS ONE 11, 4–15 (2016).
Kim, D.-H. et al. Biofunctionalized magnetic-vortex microdiscs for targeted cancer-cell destruction. Nat. Mater. 9, 165–171 (2010).
Hein, M. A. et al. Fabrication of bioinspired inorganic nanocilia sensors. IEEE Trans. Magn. 49, 191–196 (2013).
Brataas, A., Kent, A. D. & Ohno, H. Current-induced torques in magnetic materials. Nat. Mater. 11, 372–381 (2012).
Locatelli, N., Cros, V. & Grollier, J. Spin-torque building blocks. Nat. Mater. 13, 11–20 (2014).
Parkin, S. S. P., Hayashi, M. & Thomas, L. Magnetic domain-wall racetrack memory. Science 320, 190–194 (2008) A review of the development of racetrack memory, including the proposal of a vertical racetrack.
Ishigaki, T. et al. A multi-level-cell spin-transfer torque memory with series-stacked magnetotunnel junctions. In 2010 Symposium on VLSI Technology 47–48IEEE (2010).
Kazuo, K., Morihiro, K. & Kenji, T. (eds). Three-Dimensional Integration of Semiconductors Processing, Materials, and Applications (Springer, 2015).
Ono, T. H., Miyajima, K., Shigeto, K., Mibu, N. & Hosoito, T. S. Propagation of a magnetic domain wall in a submicrometer magnetic wire. Science 284, 468–470 (1999) This work shows domain wall conduit behaviour in nanowires.
Chumak, A. V., Vasyuchka, V. I., Serga, A. A. & Hillebrands, B. Magnon spintronics. Nat. Phys. 11, 453–461 (2015).
Allwood, D. A. et al. Magnetic domain-wall logic. Science 309, 1688–1692 (2005) This paper demonstrates domain wall logic based on magnetic nanowires.
Lequeux, S. et al. A magnetic synapse: multilevel spin-torque memristor with perpendicular anisotropy. Sci. Rep. 6, 31510 (2016).
Von Neumann, J., Churchland, P. M. & Churchland, P. S. The Computer And The Brain Yale University Press (2000).
Bauer, G. E. W., Saitoh, E. & van Wees, B. J. Spin caloritronics. Nat. Mater. 11, 391–399 (2012).
Fusil, S., Garcia, V., Barthélémy, A. & Bibes, M. Magnetoelectric devices for spintronics. Annu. Rev. Mater. Res. 44, 91–116 (2014).
Xu, S. et al. Materials science. Assembly of micro/nanomaterials into complex, three-dimensional architectures by compressive buckling. Science 347, 154–159 (2015).
Fisher, J. S., Kottke, P. A., Kim, S. & Fedorov, A. G. Rapid electron beam writing of topologically complex 3D nanostructures using liquid phase precursor. Nano Lett. 15, 8385–8391 (2015).
Fix, T. et al. Electric-field control of ferromagnetism in a nanocomposite via a ZnO phase. Nano Lett. 13, 5886–5890 (2013).
Rusz, J., Idrobo, J.-C. & Bhowmick, S. Achieving atomic resolution magnetic dichroism by controlling the phase symmetry of an electron probe. Phys. Rev. Lett. 113, 145501 (2014).
Guzzinati, G. et al. Prospects for versatile phase manipulation in the TEM: beyond aberration correction. Ultramicroscopy 151, 85–93 (2015).
Lutman, A. A. et al. Polarization control in an X-ray free-electron laser. Nat. Photonics 10, 468–472 (2016).
Park, H. S., Baskin, J. S. & Zewail, A. H. 4D Lorentz electron microscopy imaging: magnetic domain wall nucleation, reversal, and wave velocity. Nano Lett. 10, 3796–3803 (2010).
Gao, F. & Gu, Z. Nano-soldering of magnetically aligned three-dimensional nanowire networks. Nanotechnology 21, 115604 (2010).
Yang, S.-H., Ryu, K.-S. & Parkin, S. Domain-wall velocities of up to 750ms(-1) driven by exchange-coupling torque in synthetic antiferromagnets. Nat. Nanotechnol. 10, 221–226 (2015).
Braun, H.-B. Topological effects in nanomagnetism: from superparamagnetism to chiral quantum solitons. Adv. Phys. 61, 1–116 (2012).
Markov, I. L. Limits on fundamental limits to computation. Nature 512, 147–154 (2014).
Wang, R. F. et al. Artificial ‘spin ice’ in a geometrically frustrated lattice of nanoscale ferromagnetic islands. Nature 439, 303–306 (2006).
Donnelly, C. et al. Element-specific X-ray phase tomography of 3D structures at the nanoscale. Phys. Rev. Lett. 114, 115501 (2015).
Tottori, S. et al. Magnetic helical micromachines: fabrication, controlled swimming, and cargo transport. Adv. Mater. 24, 811–816 (2012).
Albrecht, M. et al. Magnetic multilayers on nanospheres. Nat. Mater. 4, 203–206 (2005).
Streubel, R. et al. Equilibrium magnetic states in individual hemispherical permalloy caps. Appl. Phys. Lett. 101, 132419 (2012).
Eslami, S. et al. Chiral nanomagnets. ACS Photonics 1, 1231–1236 (2014).
Gibbs, J. G. et al. Nanohelices by shadow growth. Nanoscale 6, 9457–9466 (2014).
Yannopapas, V. & Vanakaras, A. G. Strong magnetochiral dichroism in suspensions of magnetoplasmonic nanohelices. ACS Photonics 2, 1030–1038 (2015).
Schmidt, O. G. & Eberl, K. Nanotechnology: thin solid films roll up into nanotubes. Nature 410, 168–168 (2001) This brief communication describes the development of rolled-up nanotechnology.
Lara, P. et al. in Advances in Organometallic Chemistry and Catalysis: the Silver/Gold Jubilee International Conference on Organometallic Chemistry Celebratory Book ed. Pombeiro A. J. L. Ch. 31, Wiley (2014).
Anagnostopoulou, E. et al. Dense arrays of cobalt nanorods as rare-earth free permanent magnets. Nanoscale 8, 4020–4029 (2016).
Liakakos, N. et al. Solution epitaxial growth of cobalt nanowires on crystalline substrates for data storage densities beyond 1 Tbit/in2. Nano Lett. 14, 3481–3486 (2014).
Vivas, L. G., Escrig, J., Trabada, D. G., Badini-Confalonieri, G. A. & Väzquez, M. Magnetic anisotropy in ordered textured Co nanowires. Appl. Phys. Lett. 100, 252405 (2012).
Zierold, R. et al. Magnetic, multilayered nanotubes of low aspect ratios for liquid suspensions. Adv. Funct. Mater. 21, 226–232 (2011).
Ozel, T., Bourret, G. R. & Mirkin, C. A. Coaxial lithography. Nat. Nanotechnol. 10, 319–324 (2015).
Lee, J. H. et al. Iron–gold barcode nanowires. Angew. Chem. Int Ed. 46, 3663–3667 (2007).
Piraux, L. et al. Template-grown NiFe/Cu/NiFe nanowires for spin transfer devices. Nano Lett. 7, 2563–2567 (2007).
Huang, X., Tan, L., Cho, H. & Stadler, B. J. H. Magnetoresistance and spin transfer torque in electrodeposited Co/Cu multilayered nanowire arrays with small diameters. J. Appl. Phys. 105, 07D128 (2009).
Sousa, C. T. et al. Nanoporous alumina as templates for multifunctional applications. Appl. Phys. Rev. 1, 031102 (2014).
Lee, W. et al. Structural engineering of nanoporous anodic aluminium oxide by pulse anodization of aluminium. Nat. Nanotechnol. 3, 234–239 (2008).
Ross, C. A., Berggren, K. K., Cheng, J. Y., Jung, Y. S. & Chang, J.-B. Three-dimensional nanofabrication by block copolymer self-assembly. Adv. Mater. 26, 4386–4396 (2014).
Mistonov, A. A. et al. Three-dimensional artificial spin ice in nanostructured Co on an inverse opal-like lattice. Phys. Rev. B 87, 220408 (2013).
Hsueh, H.-Y. et al. Nanoporous gyroid nickel from block copolymer templates via electroless plating. Adv. Mater. 23, 3041–3046 (2011).
Utke, I., Hoffmann, P. & Melngailis, J. Gas-assisted focused electron beam and ion beam processing and fabrication. J. Vac. Sci. Technol. B Microelectron. Nanom. Struct. 26, 1197–1276 (2008).
Fernández-Pacheco, A., De Teresa, J. M., Córdoba, R. & Ibarra, M. R. Magnetotransport properties of high-quality cobalt nanowires grown by focused-electron-beam-induced deposition. J. Phys. D Appl. Phys. 42, 055005 (2009) This paper reports the 3D nano-printing of ferromagnetic nanostructures with purities above 90%.
De Teresa, J. M. et al. Review of magnetic nanostructures grown by focused electron beam induced deposition (FEBID). J. Phys. D Appl. Phys. 49, 243003 (2016).
Bernau, L., Gabureac, M., Erni, R. & Utke, I. Tunable nanosynthesis of composite materials by electron-impact reaction. Angew. Chem. 122, 9064–9068 (2010).
Porrati, F. et al. Direct writing of CoFe alloy nanostructures by focused electron beam induced deposition from a heteronuclear precursor. Nanotechnology 26, 475701 (2015).
Costanzi, B. N., Riazanova, A. V., Dan Dahlberg, E. & Belova, L. M. In situ manufacture of magnetic tunnel junctions by a direct-write process. Appl. Phys. Lett. 104, 222401 (2014).
Utke, I., Hoffmann, P., Berger, R. & Scandella, L. High-resolution magnetic Co supertips grown by a focused electron beam. Appl. Phys. Lett. 80, 4792–4794 (2002).
Fernández-Pacheco, A. et al. Three dimensional magnetic nanowires grown by focused electron-beam induced deposition. Sci. Rep. 3, 1492 (2013) This work demonstrates the magneto-optical detection of magnetic nanowires in a 3D configuration.
Takeguchi, M., Shimojo, M., Che, R. & Furuya, K. Fabrication of a nano-magnet on a piezo-driven tip in a TEM sample holder. J. Mater. Sci. 41, 2627–2630 (2006).
Lau, Y. M., Chee, P. C., Thong, J. T. L. & Ng, V. Properties and applications of cobalt-based material produced by electron-beam-induced deposition. J. Vac. Sci. Technol. A Vac. Surf. Film 20, 1295–1302 (2002).
Esposito, M. et al. Nanoscale 3D chiral plasmonic helices with circular dichroism at visible frequencies. ACS Photonics 2, 105–114 (2015).
Botman, A., Mulders, J. J. L. & Hagen, C. W. Creating pure nanostructures from electron-beam-induced deposition using purification techniques: a technology perspective. Nanotechnology 20, 372001 (2009).
Plank, H. et al. Electron-beam-assisted oxygen purification at low temperatures for electron-beam-induced pt deposits: towards pure and high-fidelity nanostructures. ACS Appl. Mater. Interfaces 6, 1018–1024 (2014).
Roberts, N. A., Fowlkes, J. D., Magel, G. A. & Rack, P. D. Enhanced material purity and resolution via synchronized laser assisted electron beam induced deposition of platinum. Nanoscale 5, 408–415 (2013).
Fowlkes, J. D. Simulation guided 3D nanomanufacturing via focused electron beam induced deposition. ACS Nano 10, 6163–6172 (2016) This article presents the 3D nano-printing of complex nanostructures making use of modelling based on Monte Carlo and continuum model methods.
Wernsdorfer, W. et al. Nucleation of magnetization reversal in individual nanosized nickel wires. Phys. Rev. Lett. 77, 1873–1876 (1996).
Allwood, D. a., Xiong, G., Cooke, M. D. & Cowburn, R. P. Magneto-optical Kerr effect analysis of magnetic nanostructures. J. Phys. D Appl. Phys. 36, 2175–2182 (2003).
Jaafar, M. et al. Hysteresis loops of individual Co nanostripes measured by magnetic force microscopy. Nanoscale Res. Lett. 6, 407 (2011).
Weber, D. P. et al. Cantilever magnetometry of individual Ni nanotubes. Nano Lett. 12, 6139–6144 (2012).
Buchter, A. et al. Reversal mechanism of an individual Ni nanotube simultaneously studied by torque and SQUID magnetometry. Phys. Rev. Lett. 111, 067202 (2013).
Banerjee, P. et al. Magnetization reversal in an individual 25 nm iron-filled carbon nanotube. Appl. Phys. Lett. 96, 252505 (2010).
Fitzsimmons, M. R. & Schuller, I. K. Neutron scattering—the key characterization tool for nanostructured magnetic materials. J. Magn. Magn. Mater. 350, 199–208 (2014).
Adams, T. et al. Long-wavelength helimagnetic order and skyrmion lattice phase in Cu 2 OSeO 3. Phys. Rev. Lett. 108, 237204 (2012).
Tokunaga, Y. et al. A new class of chiral materials hosting magnetic skyrmions beyond room temperature. Nat. Commun. 6, 7638 (2015).
Manke, I. et al. Three-dimensional imaging of magnetic domains. Nat. Commun. 1, 125 (2010).
Maurer, T. et al. Ordered arrays of magnetic nanowires investigated by polarized small-angle neutron scattering. Phys. Rev. B 89, 184423 (2014).
Fischer, P. X-ray imaging of magnetic structures. IEEE Trans. Magn. 51, 1–31 (2015).
Reyes, D., Biziere, N., Warot-Fonrose, B., Wade, T. & Gatel, C. Magnetic configurations in Co/Cu multilayered nanowires: evidence of structural and magnetic interplay. Nano Lett. 16, 1230–1236 (2016).
Yu, X. Z. et al. Real-space observation of a two-dimensional skyrmion crystal. Nature 465, 901–904 (2010).
Zhao, X. et al. Direct imaging of magnetic field-driven transitions of skyrmion cluster states in FeGe nanodisks. Proc. Natl Acad. Sci. USA 113, 4918–4923 (2016).
Ivanov, Y. P., Chuvilin, A., Lopatin, S. & Kosel, J. Modulated magnetic nanowires for controlling domain wall motion: toward 3D magnetic memories. ACS Nano 10, 5326–5332 (2016).
Midgley, P. A. & Dunin-Borkowski, R. E. Electron tomography and holography in materials science. Nat. Mater. 8, 271–280 (2009).
Phatak, C., Tanase, M., Petford-Long, A. K. & De Graef, M. Determination of magnetic vortex polarity from a single Lorentz Fresnel image. Ultramicroscopy 109, 264–267 (2009).
Wolf, D. et al. 3D magnetic induction maps of nanoscale materials revealed by electron holographic tomography. Chem. Mater. 27, 6771–6778 (2015).
Simon, P. et al. Synthesis and three-dimensional magnetic field mapping of Co2 FeGa Heusler nanowires at 5 nm resolution. Nano Lett. 16, 114–120 (2016).
Phatak, C. et al. Visualization of the magnetic structure of sculpted three-dimensional cobalt nanospirals. Nano Lett. 14, 759–764 (2014).
Phatak, C. et al. Quantitative 3D electromagnetic field determination of 1D nanostructures from single projection. Ultramicroscopy 164, 24–30 (2016).
Phatak, C., Petford-Long, A. K. & De Graef, M. Three-dimensional study of the vector potential of magnetic structures. Phys. Rev. Lett. 104, 253901 (2010) This paper demonstrates three-dimensional magnetic vectorial tomography using electron microscopy.
Tanigaki, T. et al. Three-dimensional observation of magnetic vortex cores in stacked ferromagnetic discs. Nano Lett. 15, 1309–1314 (2015).
Kimling, J. et al. Photoemission electron microscopy of three-dimensional magnetization configurations in core-shell nanostructures. Phys. Rev. B 84, 174406 (2011).
Streubel, R. et al. Retrieving spin textures on curved magnetic thin films with full-field soft X-ray microscopies. Nat. Commun. 6, 7612 (2015) This work demonstrates three-dimensonal magnetic vectorial tomography using X-ray microscopy.
Streubel, R. et al. Imaging of buried 3D magnetic rolled-up nanomembranes. Nano Lett. 14, 3981–3986 (2014).
Blanco-Roldán, C. et al. Nanoscale imaging of buried topological defects with quantitative X-ray magnetic microscopy. Nat. Commun. 6, 8196 (2015).
Hertel, R. et al. Three-dimensional magnetic-flux-closure patterns in mesoscopic Fe islands. Phys. Rev. B 72, 214409 (2005).
Kakay, A., Westphal, E. & Hertel, R. Speedup of FEM micromagnetic simulations with graphical processing units. IEEE Trans. Magn. 46, 2303–2306 (2010).
Shaojing, L., Livshitz, B. & Lomakin, V. Graphics processing unit accelerated O(N) micromagnetic solver. IEEE Trans. Magn. 46, 2373–2375 (2010).
Sato, T. & Nakatani, Y. Fast micromagnetic simulation of vortex core motion by GPU. J. Magn. Soc. Jpn 35, 163–170 (2011).
Kittel, C. Physical theory of ferromagnetic domains. Rev. Mod. Phys. 21, 541–583 (1949).
Andreas, C., Gliga, S. & Hertel, R. Numerical micromagnetism of strong inhomogeneities. J. Magn. Magn. Mater. 362, 7–13 (2014).
Evans, R. F. L. et al. Atomistic spin model simulations of magnetic nanomaterials. J. Phys. Condens. Matter 26, 103202 (2014).
Bergqvist, L., Taroni, A., Bergman, A., Etz, C. & Eriksson, O. Atomistic spin dynamics of low-dimensional magnets. Phys. Rev. B 87, 144401 (2013).
This work has received funding from the European Union Seventh Framework Programme (FP7/2007-2013) under grant agreements no. 309589: M3d, and no. 247368: 3SPIN. A.F-P. acknowledges support from an EPSRC Early Career Fellowship, EP/M008517/1 and from a Winton Fellowship. R.S. and P.F. acknowledge support by the U.S. Department of Energy, Office of Science, Office of Basic Energy Sciences, Materials Sciences and Engineering Division, under contract no. DE-AC02-05-CH11231 within the Non-Equilibrium Magnetic Materials programme (MSMAG). We thank Alexander Welbourne for proofreading the manuscript.
The authors declare no competing financial interests.
About this article
Cite this article
Fernández-Pacheco, A., Streubel, R., Fruchart, O. et al. Three-dimensional nanomagnetism. Nat Commun 8, 15756 (2017). https://doi.org/10.1038/ncomms15756
Journal of Colloid and Interface Science (2021)
Harnessing Multi-Photon Absorption to Produce Three-Dimensional Magnetic Structures at the Nanoscale
Physical Review B (2020)
ACS Applied Nano Materials (2020)